Transformation of a layered perovskite to a defect perovskite via cooperative Li-insertion and O/N substitution.
Kim, Jung-Mi; Kim, Young-Il; Park, Chee-Sung; Park, Cheol-Hee; Dalton transactions (Cambridge, England : 2003) 43 (2014) 16830–16837; doi:10.1039/c4dt02335h

data_7032562
_publ_section_title
;
 Transformation of a layered perovskite to a defect perovskite via
 cooperative Li-insertion and O/N substitution.
;
_journal_issue                   44
_journal_name_full
'Dalton transactions (Cambridge, England : 2003)'
_journal_page_first              16830
_journal_page_last               16837
_journal_paper_doi               10.1039/c4dt02335h
_journal_volume                  43
_journal_year                    2014
_chemical_formula_sum            'Li0.32 N3.56 O7.64 Sr3.68 Ta3.68'
_chemical_formula_weight         1162.65
_chemical_name_systematic        ' ?'
_space_group_IT_number           140
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4 2c'
_symmetry_space_group_name_H-M   'I 4/m c m'
_audit_creation_date             2014-07-31T15:01
_audit_creation_method           'from EXP file using GSAS2CIF'
_audit_update_record
' 2014-07-31T15:01  Initial CIF as created by GSAS2CIF'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                90.0
_cell_formula_units_Z            1
_cell_length_a                   5.69719(4)
_cell_length_b                   5.69719
_cell_length_c                   8.07118(12)
_cell_volume                     261.974(4)
_computing_structure_refinement  GSAS
_diffrn_radiation_polarisn_ratio 0.573
_diffrn_radiation_probe          x-ray
_diffrn_radiation_wavelength     1.5406
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  1.00000
_exptl_absorpt_process_details
;   GSAS Absorption/surface roughness correction: function number 0
 No correction is applied.
;
_pd_block_id                     2014-07-31T15:01|LI01CIF|Young-Il_Kim|BrukerD8
_pd_calc_method                  'Rietveld Refinement'
_pd_instr_location               ' ?'
_pd_meas_number_of_points        8168
_pd_phase_name                   I4/mcm
_pd_proc_info_datetime           2014-07-31T15:01:12
_pd_proc_info_excluded_regions   ' ?'
_pd_proc_ls_background_function
;   GSAS Background function number 7 with 16 terms.
 Linear interpolation
      1:    105.215     2:    117.461     3:    102.092     4:    93.9398    
      5:    80.2658     6:    103.655     7:    67.8579     8:    77.2109    
      9:    79.1455    10:    78.8191    11:    84.7801    12:    79.4221    
     13:    95.0330    14:    114.851    15:    124.708    16:    131.579    
;
_pd_proc_ls_peak_cutoff          0.00050
_pd_proc_ls_pref_orient_corr
;   March-Dollase
 AXIS  1 Ratio=     0.859 Frac     0.500  h= 0.000  k= 0.000  l= 1.000
 AXIS  2 Ratio=     0.736 Frac     0.500  h= 1.000  k= 0.000  l= 0.000
 Prefered orientation correction range: Min=   0.92355, Max=   1.18233
;
_pd_proc_ls_profile_function
;
 CW Profile function number 3 with  19 terms
 Pseudovoigt profile coefficients as parameterized in
 P. Thompson, D.E. Cox & J.B. Hastings (1987). J. Appl. Cryst.,20,79-83.
 Asymmetry correction of L.W. Finger, D.E. Cox & A. P. Jephcoat (1994).
 J. Appl. Cryst.,27,892-900.
 Peak tails are ignored  where the intensity is below 0.0005 times the peak
   Aniso. broadening axis   0.0   0.0   1.0
;
_pd_proc_ls_prof_R_factor        0.0585
_pd_proc_ls_prof_wR_expected     0.0457
_pd_proc_ls_prof_wR_factor       0.0834
_pd_proc_number_of_points        8168
_pd_spec_mounting                ' ?'
_refine_ls_goodness_of_fit_all   1.83
_refine_ls_matrix_type           full
_refine_ls_number_parameters     30
_refine_ls_number_restraints     0
_refine_ls_R_Fsqd_factor         0.02025
_refine_ls_shift/su_max          0.02
_refine_ls_shift/su_mean         0.00
_reflns_d_resolution_high        0.806
_reflns_d_resolution_low         4.036
_reflns_limit_h_max              7
_reflns_limit_h_min              0
_reflns_limit_k_max              5
_reflns_limit_k_min              0
_reflns_limit_l_max              10
_reflns_limit_l_min              0
_reflns_number_total             85
_cod_data_source_file            c4dt02335h1.cif
_cod_data_source_block           LI01CIF_publ
_cod_depositor_comments
;
The following automatic conversions were performed:

'_geom_bond_publ_flag' value 'N' changed to 'n' according to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26 (118
times).

'_geom_angle_publ_flag' value 'N' changed to 'n' according
to
/usr/data/users/saulius/crontab/automatic-downloads/rss-feeds/RSC/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 from 2011-04-26 (792
times).

Automatic conversion script
Id: cif_fix_values 2281 2013-09-26 08:29:07Z andrius 

 Adding full bibliography for 7032562--7032565.cif.
;
_cod_original_cell_volume        261.9740(30)
_cod_database_code               7032562
_gsas_exptl_extinct_corr_t_min   1.00000
_gsas_exptl_extinct_corr_t_max   1.00000